data_global 
_audit_creation_date        "11-06-20"
_audit_creation_method CRYSTALS_ver_14.11

_oxford_structure_analysis_title  'Bu3_12 in C2/c'
_chemical_name_systematic         '2M1 phlogopite'
_chemical_melting_point           ?


data_1 

_publ_requested_journal          Am.Miner.
_publ_contact_author_name        'Professor Fernando Scordari '
_publ_contact_author_address     
;Dipartimento Geomineralogico 
Universita' di Bari 
Via Orabona 4 
I-70125 Bari 
Italy
;
_publ_contact_author_email       f.scordari@geomin.uniba.it
_publ_contact_author_phone       '+39 080 5442587'
_publ_contact_author_fax         '+39 080 5442597'

_publ_section_title 
; 
CRYSTAL CHEMISTRY OF TRIOCTAHEDRAL MICAS-2M1 FROM BUNYARUGURU 
(SW UGANDA) KAMAFUGITE 
; 


loop_
_publ_author_name
_publ_author_address
'Scordari, Fernando '
;Dipartimento Geomineralogico 
Universita' di Bari 
Via Orabona 4 
I-70125 Bari 
Italy
;
'Schingaro, Emanuela'
;Dipartimento Geomineralogico 
Universita' di Bari 
Via Orabona 4 
I-70125 Bari 
Italy
;
'Lacalamita, Maria'
;Dipartimento Geomineralogico 
Universita' di Bari 
Via Orabona 4 
I-70125 Bari 
Italy
;
'Mesto, Ernesto'
;Dipartimento Geomineralogico 
Universita' di Bari 
Via Orabona 4 
I-70125 Bari 
Italy
;
 
_cell_length_a                    5.33070(10)
_cell_length_b                    9.2315(3)
_cell_length_c                    20.1550(6)
_cell_angle_alpha                 90
_cell_angle_beta                  95.095(2)
_cell_angle_gamma                 90
_cell_volume                      987.92(5)
 
_symmetry_cell_setting            'Monoclinic' 
_symmetry_space_group_name_H-M    'C 1 2/c 1 ' 
_symmetry_space_group_name_Hall   ? 
loop_
 _symmetry_equiv_pos_as_xyz
 'x,y,z'
 '-x,-y,-z'
 'x+1/2,y+1/2,z'
 '-x+1/2,-y+1/2,-z'
 '-x,y,-z+1/2'
 'x,-y,z+1/2'
 '-x+1/2,y+1/2,-z+1/2'
 'x+1/2,-y+1/2,z+1/2'

loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source  
 H       0.0000   0.0000   0.4930  10.5109   0.3229  26.1257   0.1402   3.1424
   0.0408  57.7997   0.0030 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
 Fep2    0.3010   0.8450  11.0424   4.6538   7.3740   0.3053   4.1346  12.0546
   0.4399  31.2809   1.0097 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
 Kp1     0.1790   0.2500   7.9578  12.6331   7.4917   0.7674   6.3590  -0.0020
   1.1915  31.9128  -4.9978 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
 Mgp2    0.0420   0.0360   3.4988   2.1676   3.8378   4.7542   1.3284   0.1850
   0.8497  10.1411   0.4853 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
 Si      0.0720   0.0710   6.2915   2.4386   3.0353  32.3337   1.9891   0.6785
   1.5410  81.6937   1.1407 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
 Sip4    0.0720   0.0710   4.4392   1.6417   3.2034   3.4376   1.1945   0.2149
   0.4165   6.6536   0.7463 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
 O       0.0080   0.0060   3.0485  13.2771   2.2868   5.7011   1.5463   0.3239
   0.8670  32.9089   0.2508 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
 Om2     0.0080   0.0060   3.7504  16.5151   2.8429   6.5920   1.5430   0.3192
   1.6209  43.3486   0.2421 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
 
 
_cell_formula_units_Z                    4

# Given Formula = H2 Fep21.50 Kp11 Mgp21.50 O6 Om26 Sip42 Si2 
# Dc =      3.13 Fooo =    830.72 Mu =     55.26 M =    232.84
# Found Formula = Fep20.74 Kp10.50 Mgp21.76 O3.61 Om28.39 Si2.62 Sip41.38 
# Dc =      2.99 FOOO =    830.72 Mu =     50.61 M =    222.11

_chemical_formula_sum             'Fep20.74 Kp10.50 Mgp21.76 O3.61 Om28.39 Si2.62 Sip41.38'
_chemical_formula_moiety          'Fep20.74 Kp10.50 Mgp21.76 O3.61 Om28.39 Si2.62 Sip41.38'
_chemical_compound_source         'Natural'
_chemical_formula_weight            444.23
 
 
_cell_measurement_reflns_used            0
_cell_measurement_theta_min              0
_cell_measurement_theta_max              0
_cell_measurement_temperature          293
 
_exptl_crystal_description        'platy' 
_exptl_crystal_colour             'brown' 
_exptl_crystal_size_min           0.010 
_exptl_crystal_size_mid           0.150		
_exptl_crystal_size_max           0.410 
 
_exptl_crystal_density_diffrn     2.987 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_method     'not measured' 
# Non-dispersive F(000): 
_exptl_crystal_F_000              830.721 
_exptl_absorpt_coefficient_mu     5.061 
 
# Sheldrick geometric approximatio 1.00 0.95 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_process_details    'SADABS (Siemens, 1996)' 
_exptl_absorpt_correction_T_min   0.7438 
_exptl_absorpt_correction_T_max   1.0000 
# For a Kappa CCD, set Tmin to 1.0 and 
# Tmax to the ratio of max:min frame scales in scale_all.log 
_diffrn_measurement_device_type   'Nonius KappaCCD' 
_diffrn_measurement_device        'Area' 
_diffrn_radiation_monochromator   'graphite' 
_diffrn_radiation_type            'Mo K\a'
_diffrn_radiation_wavelength           0.71073
_diffrn_measurement_method        ω/2θ 
 
# If a reference occurs more than once, delete the author 
# and date from subsequent references. 
_computing_data_collection        'COLLECT (Nonius, 2001).' 
_computing_cell_refinement        'DENZO/SCALEPACK (Otwinowski & Minor, 1997)' 
_computing_data_reduction         'DENZO/SCALEPACK (Otwinowski & Minor, 1997)' 
_computing_structure_solution     'Superflip (Palatinus & Chapuis, 2007)' 
_computing_structure_refinement   'CRYSTALS (Betteridge et al., 2003)' 
_computing_publication_material   'CRYSTALS (Betteridge et al., 2003)' 
_computing_molecular_graphics     'CAMERON (Watkin et al., 1996)' 
 
_diffrn_standards_interval_time   . 
_diffrn_standards_interval_count  . 
_diffrn_standards_number          0 
_diffrn_standards_decay_%         ? 
 
_diffrn_ambient_temperature        293
_diffrn_reflns_number             14015 
_reflns_number_total              2800 
_diffrn_reflns_av_R_equivalents   0.035 
# Number of reflections without Friedels Law is 2800 
# Number of reflections with Friedels Law is 0 
# Theoretical number of reflections is about 2792 
 
 
_diffrn_reflns_theta_min          4.060 
_diffrn_reflns_theta_max          38.563 
_diffrn_measured_fraction_theta_max 0.998 
 
_diffrn_reflns_theta_full         38.563 
_diffrn_measured_fraction_theta_full 0.998 
 
 
_diffrn_reflns_limit_h_min        -9 
_diffrn_reflns_limit_h_max        9 
_diffrn_reflns_limit_k_min        -15 
_diffrn_reflns_limit_k_max        16 
_diffrn_reflns_limit_l_min        -35 
_diffrn_reflns_limit_l_max        35 
_reflns_limit_h_min               -9 
_reflns_limit_h_max               9 
_reflns_limit_k_min               0 
_reflns_limit_k_max               16 
_reflns_limit_l_min               0 
_reflns_limit_l_max               35 
 
_oxford_diffrn_Wilson_B_factor    0.00 
_oxford_diffrn_Wilson_scale       0.00 
 
_atom_sites_solution_primary      direct #heavy,direct,difmap,geom
# _atom_sites_solution_secondary  difmap
_atom_sites_solution_hydrogens    geom
 
_refine_diff_density_min          -0.54 
_refine_diff_density_max          0.91 
 
 
# The current dictionary definitions do not cover the 
# situation where the reflections used for refinement were 
# selected by a user-defined sigma threshold 
 
 
# The values actually used during refinement 
_oxford_reflns_threshold_expression_ref     I>3.0\s(I)
_refine_ls_number_reflns          1394 
_refine_ls_number_restraints      24 
_refine_ls_number_parameters      106 
_oxford_refine_ls_R_factor_ref    0.0291 
_refine_ls_wR_factor_ref          0.0291 
_refine_ls_goodness_of_fit_ref    0.9817 
_refine_ls_shift/su_max           0.0106609 
_refine_ls_shift/su_mean          0.0002795 
 
 
# The values computed from all data 
_oxford_reflns_number_all         2653 
_refine_ls_R_factor_all           0.0771 
_refine_ls_wR_factor_all          0.0575 
 
# The values computed with a 2 sigma cutoff - a la SHELX 
_reflns_threshold_expression      I>2.0σ(I)
_reflns_number_gt                 1549 
_refine_ls_R_factor_gt            0.0365 
_refine_ls_wR_factor_gt           0.0316 
 
# choose from: rm (reference molecule of known chirality), 
# ad (anomolous dispersion - Flack), rmad (rm and ad), 
# syn (from synthesis), unk (unknown) or . (not applicable). 
_chemical_absolute_configuration  '.' 
 
 
_refine_ls_structure_factor_coef  F 
_refine_ls_matrix_type            full
_refine_ls_hydrogen_treatment     none           # none, undef, noref, refall,
                                                 # refxyz, refU, constr or mixed
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
;
 Method, part 1, Chebychev polynomial, (Watkin, 1994, Prince, 1982) 
 [weight] = 1.0/[A₀*T₀(x)+A₁*T₁(x) ... +Aₙ₋₁]*Tₙ₋₁(x)] 
 where Ai are the Chebychev coefficients listed below and x= Fcalc/Fmax 
 Method = Robust Weighting (Prince, 1982) 
 W = [weight] * [1-(deltaF/6*sigmaF)²]² 
 Ai are: 
 0.252 0.226 0.184 0.746E-01 0.425E-01 
;
# Insert your own references if required - in alphabetical order 
_publ_section_references 
; 
Betteridge, P.W., Carruthers, J.R., Cooper, R.I., 
Prout, K. & Watkin, D.J. (2003). J. Appl. Cryst. 36, 1487. 
 
Nonius (2001). COLLECT. Nonius BV, Delft, The Netherlands. 
 
Otwinowski, Z. & Minor, W. (1997). Methods in Enzymology, Vol. 276, 
edited by C. W. Carter Jr & R. M. Sweet, pp. 307--326. 
New York: Academic Press. 
 
Palatinus, L. & Chapuis, G. (2007). J. Appl. Cryst. 40, 786-790. 
 
Prince, E. 
Mathematical Techniques in Crystallography 
and Materials Science 
Springer-Verlag, New York, 1982. 
 
Siemens Industrial Automation, Inc (1996). 
SADABS: Area-Detector Absorption Correction;: Madison, WI. 
 
Watkin D.J. (1994). 
Acta Cryst, A50, 411-437. 
 
Watkin, D.J., Prout, C.K. & Pearce, L.J. (1996). CAMERON, Chemical 
Crystallography Laboratory, Oxford, UK. 
; 

# Uequiv = arithmetic mean of Ui i.e. Ueqiv = (U1+U2+U3)/3

# Replace last . with number of unfound hydrogen atomsattached to an atom.

# ..._refinement_flags_... 
# . no refinement constraints           S special position constraint on site
# G rigid group refinement of site      R riding atom
# D distance or angle restraint on site T thermal displacement constraints
# U Uiso or Uij restraint (rigid bond)  P partial occupancy constraint


loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
_atom_site_attached_hydrogens
Kp11 Kp1 0.0000 0.08397(13) 0.2500 0.0362 1.0069(9) Uani . . P . . . 
Mgp22 Mgp2 0.7500 0.2500 0.0000 0.0119 0.7288(8) Uani . . P . . . 
Fep22 Fep2 0.7500 0.2500 0.0000 0.0119 0.2714(7) Uani . . P . . . 
Mgp23 Mgp2 0.24036(9) 0.08007(6) -0.00003(2) 0.0137 0.6982(8) Uani . . P . . . 
Fep23 Fep2 0.24036(9) 0.08007(6) -0.00003(2) 0.0137 0.3018(8) Uani . . P . . . 
Sip44 Sip4 0.46197(10) 0.25017(6) 0.13724(3) 0.0103 0.3962(7) Uani . . P . . . 
Si4 Si 0.46197(10) 0.25017(6) 0.13724(3) 0.0103 0.6038(7) Uani . . P . . . 
Sip45 Sip4 0.96326(9) 0.41742(8) 0.13725(3) 0.0111 0.2941(7) Uani . . P . . . 
Si5 Si 0.96326(9) 0.41742(8) 0.13725(3) 0.0111 0.7059(7) Uani . . P . . . 
Om26 Om2 0.7395(3) 0.31643(19) 0.16557(9) 0.0195 0.4386(7) Uani . . P . . . 
O6 O 0.7395(3) 0.31643(19) 0.16557(9) 0.0195 0.5614(7) Uani . . P . . . 
Om27 Om2 0.2391(3) 0.3503(2) 0.16642(9) 0.0199 0.4980(7) Uani . . P . . . 
O7 O 0.2391(3) 0.3503(2) 0.16642(9) 0.0199 0.5023(7) Uani . . P . . . 
Om28 Om2 0.4384(3) 0.08381(19) 0.16630(7) 0.0196 0.6372(7) Uani . . P . . . 
O8 O 0.4384(3) 0.08381(19) 0.16630(7) 0.0196 0.3629(7) Uani . . P . . . 
Om29 Om2 0.4321(2) 0.24076(18) 0.05452(7) 0.0090 0.8683(7) Uani . . P . . . 
O9 O 0.4321(2) 0.24076(18) 0.05452(7) 0.0090 0.1316(7) Uani . . P . . . 
Om210 Om2 0.9369(2) 0.4089(2) 0.05457(7) 0.0097 0.7821(7) Uani . . P . . . 
O10 O 0.9369(2) 0.4089(2) 0.05457(7) 0.0097 0.2179(7) Uani . . P . . . 
Om211 Om2 0.9343(2) 0.07332(18) 0.05103(7) 0.0102 0.9721(7) Uani . . P . . . 
O11 O 0.9343(2) 0.07332(18) 0.05103(7) 0.0102 0.0279(7) Uani . . P . . . 

_refine_ls_extinction_method 
    'None'
_oxford_refine_ls_scale 0.09090(14) 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_site_symmetry_1
 _geom_bond_atom_site_label_2
 _geom_bond_site_symmetry_2
 _geom_bond_distance
 _geom_bond_publ_flag
Mgp22 . O10 4_655 2.0392(16)    yes
Mgp22 . Om210 4_655 2.0392(16)    yes
Mgp22 . O9 4_655 2.1017(14)    yes
Mgp22 . Om29 4_655 2.1017(14)    yes
Mgp22 . Om211 4_655 2.1223(16)    yes
Mgp22 . O11 4_655 2.1223(16)    yes
Mgp22 . Fep23 1_655 3.0486(4)    yes
Mgp22 . Fep23 4_555 3.0486(4)    yes
Mgp22 . Fep23 4_655 3.1371(5)    yes
Mgp22 . Om29 . 2.1017(14)    yes
Mgp22 . O9 . 2.1017(14)    yes
Mgp22 . Om210 . 2.0392(16)    yes
Mgp22 . O10 . 2.0392(16)    yes
Mgp22 . Om211 . 2.1223(16)    yes
Mgp22 . O11 . 2.1223(16)    yes
Fep22 . O11 4_655 2.1223(16)    yes
Fep22 . Om211 4_655 2.1223(16)    yes
Fep22 . Om29 4_655 2.1017(14)    yes
Fep22 . O9 4_655 2.1017(14)    yes
Fep22 . Om210 4_655 2.0392(16)    yes
Fep22 . O10 4_655 2.0392(16)    yes
Fep22 . Fep23 1_655 3.0486(4)    yes
Fep22 . Fep23 4_555 3.0486(4)    yes
Fep22 . Fep23 4_655 3.1371(5)    yes
Fep22 . Mgp23 1_655 3.0486(4)    yes
Fep22 . Mgp23 4_555 3.0486(4)    yes
Fep22 . Mgp23 4_655 3.1371(5)    yes
Fep22 . Sip44 . 3.2807(6)    yes
Fep22 . Si4 . 3.2807(6)    yes
Fep22 . Sip45 . 3.2825(6)    yes
Fep22 . Si5 . 3.2825(6)    yes
Fep22 . Om29 . 2.1017(14)    yes
Fep22 . O9 . 2.1017(14)    yes
Fep22 . Om210 . 2.0392(16)    yes
Fep22 . O10 . 2.0392(16)    yes
Fep22 . Om211 . 2.1223(16)    yes
Fep22 . O11 . 2.1223(16)    yes
Mgp23 . Om211 2_655 1.9388(16)    yes
Mgp23 . O11 2_655 1.9388(16)    yes
Mgp23 . O11 1_455 2.0056(14)    yes
Mgp23 . Om211 1_455 2.0056(14)    yes
Mgp23 . O10 4_655 2.1250(13)    yes
Mgp23 . Om210 4_655 2.1250(13)    yes
Mgp23 . O10 3_445 2.1451(17)    yes
Mgp23 . Om210 3_445 2.1451(17)    yes
Mgp23 . O9 4_555 2.1466(16)    yes
Mgp23 . Om29 4_555 2.1466(16)    yes
Mgp23 . Fep23 2_555 2.9585(10)    yes
Mgp23 . Om29 . 2.0626(17)    yes
Mgp23 . O9 . 2.0626(17)    yes
Fep23 . O9 4_555 2.1466(16)    yes
Fep23 . Om29 4_555 2.1466(16)    yes
Fep23 . Om210 3_445 2.1451(17)    yes
Fep23 . O10 3_445 2.1451(17)    yes
Fep23 . O10 4_655 2.1250(13)    yes
Fep23 . Om210 4_655 2.1250(13)    yes
Fep23 . Fep23 2_555 2.9585(10)    yes
Fep23 . O11 1_455 2.0056(14)    yes
Fep23 . Om211 1_455 2.0056(14)    yes
Fep23 . Om211 2_655 1.9388(16)    yes
Fep23 . Om29 . 2.0626(17)    yes
Fep23 . O9 . 2.0626(17)    yes
Sip44 . Si5 1_455 3.0744(8)    yes
Sip44 . Sip45 1_455 3.0744(8)    yes
Sip44 . Sip45 . 3.0862(8)    yes
Sip44 . Si5 . 3.0862(8)    yes
Sip44 . Om26 . 1.6548(17)    yes
Sip44 . O6 . 1.6548(17)    yes
Sip44 . Om27 . 1.6540(18)    yes
Sip44 . O7 . 1.6540(18)    yes
Sip44 . Om28 . 1.6523(19)    yes
Sip44 . O8 . 1.6523(19)    yes
Sip44 . Om29 . 1.6630(16)    yes
Sip44 . O9 . 1.6630(16)    yes
Si4 . Si5 1_455 3.0744(8)    yes
Si4 . Sip45 1_455 3.0744(8)    yes
Si4 . Sip45 . 3.0862(8)    yes
Si4 . Si5 . 3.0862(8)    yes
Si4 . Om26 . 1.6548(17)    yes
Si4 . O6 . 1.6548(17)    yes
Si4 . Om27 . 1.6540(18)    yes
Si4 . O7 . 1.6540(18)    yes
Si4 . Om28 . 1.6523(19)    yes
Si4 . O8 . 1.6523(19)    yes
Si4 . Om29 . 1.6630(16)    yes
Si4 . O9 . 1.6630(16)    yes
Sip45 . Om27 1_655 1.6548(17)    yes
Sip45 . O7 1_655 1.6548(17)    yes
Sip45 . Om28 3_555 1.6534(19)    yes
Sip45 . O8 3_555 1.6534(19)    yes
Sip45 . Om26 . 1.6550(17)    yes
Sip45 . O6 . 1.6550(17)    yes
Sip45 . Om210 . 1.6617(15)    yes
Sip45 . O10 . 1.6617(15)    yes
Si5 . Om27 1_655 1.6548(17)    yes
Si5 . O7 1_655 1.6548(17)    yes
Si5 . Om28 3_555 1.6534(19)    yes
Si5 . O8 3_555 1.6534(19)    yes
Si5 . Om26 . 1.6550(17)    yes
Si5 . O6 . 1.6550(17)    yes
Si5 . Om210 . 1.6617(15)    yes
Si5 . O10 . 1.6617(15)    yes
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_site_symmetry_1
 _geom_angle_atom_site_label_2
 _geom_angle_site_symmetry_2
 _geom_angle_atom_site_label_3
 _geom_angle_site_symmetry_3
 _geom_angle
 _geom_angle_publ_flag
O10 4_655 Mgp22 . O9 4_655 97.19(6)    yes
Om210 4_655 Mgp22 . O9 4_655 97.19(6)    yes
O10 4_655 Mgp22 . Om29 4_655 97.19(6)    yes
Om210 4_655 Mgp22 . Om29 4_655 97.19(6)    yes
O10 4_655 Mgp22 . Om211 4_655 96.22(5)    yes
Om210 4_655 Mgp22 . Om211 4_655 96.22(5)    yes
O9 4_655 Mgp22 . Om211 4_655 94.33(6)    yes
Om29 4_655 Mgp22 . Om211 4_655 94.33(6)    yes
O10 4_655 Mgp22 . O11 4_655 96.22(5)    yes
Om210 4_655 Mgp22 . O11 4_655 96.22(5)    yes
O9 4_655 Mgp22 . O11 4_655 94.33(6)    yes
Om29 4_655 Mgp22 . O11 4_655 94.33(6)    yes
O10 4_655 Mgp22 . Fep23 1_655 90.44(4)    yes
Om210 4_655 Mgp22 . Fep23 1_655 90.44(4)    yes
O9 4_655 Mgp22 . Fep23 1_655 44.73(4)    yes
Om29 4_655 Mgp22 . Fep23 1_655 44.73(4)    yes
Om211 4_655 Mgp22 . Fep23 1_655 139.07(4)    yes
O10 4_655 Mgp22 . Fep23 4_555 89.56(4)    yes
Om210 4_655 Mgp22 . Fep23 4_555 89.56(4)    yes
O9 4_655 Mgp22 . Fep23 4_555 135.27(4)    yes
Om29 4_655 Mgp22 . Fep23 4_555 135.27(4)    yes
Om211 4_655 Mgp22 . Fep23 4_555 40.93(4)    yes
O10 4_655 Mgp22 . Fep23 4_655 137.84(4)    yes
Om210 4_655 Mgp22 . Fep23 4_655 137.84(4)    yes
O9 4_655 Mgp22 . Fep23 4_655 40.65(4)    yes
Om29 4_655 Mgp22 . Fep23 4_655 40.65(4)    yes
Om211 4_655 Mgp22 . Fep23 4_655 88.82(4)    yes
O10 4_655 Mgp22 . Om29 . 82.81(6)    yes
Om210 4_655 Mgp22 . Om29 . 82.81(6)    yes
O9 4_655 Mgp22 . Om29 . 179.995    yes
Om29 4_655 Mgp22 . Om29 . 179.995    yes
Om211 4_655 Mgp22 . Om29 . 85.67(6)    yes
O10 4_655 Mgp22 . O9 . 82.81(6)    yes
Om210 4_655 Mgp22 . O9 . 82.81(6)    yes
O9 4_655 Mgp22 . O9 . 179.995    yes
Om29 4_655 Mgp22 . O9 . 179.995    yes
Om211 4_655 Mgp22 . O9 . 85.67(6)    yes
O10 4_655 Mgp22 . Om210 . 179.994    yes
Om210 4_655 Mgp22 . Om210 . 179.994    yes
O9 4_655 Mgp22 . Om210 . 82.81(6)    yes
Om29 4_655 Mgp22 . Om210 . 82.81(6)    yes
Om211 4_655 Mgp22 . Om210 . 83.78(5)    yes
O10 4_655 Mgp22 . O10 . 179.994    yes
Om210 4_655 Mgp22 . O10 . 179.994    yes
O9 4_655 Mgp22 . O10 . 82.81(6)    yes
Om29 4_655 Mgp22 . O10 . 82.81(6)    yes
Om211 4_655 Mgp22 . O10 . 83.78(5)    yes
O10 4_655 Mgp22 . Om211 . 83.78(5)    yes
Om210 4_655 Mgp22 . Om211 . 83.78(5)    yes
O9 4_655 Mgp22 . Om211 . 85.67(6)    yes
Om29 4_655 Mgp22 . Om211 . 85.67(6)    yes
Om211 4_655 Mgp22 . Om211 . 179.995    yes
O10 4_655 Mgp22 . O11 . 83.78(5)    yes
Om210 4_655 Mgp22 . O11 . 83.78(5)    yes
O9 4_655 Mgp22 . O11 . 85.67(6)    yes
Om29 4_655 Mgp22 . O11 . 85.67(6)    yes
Om211 4_655 Mgp22 . O11 . 179.995    yes
O11 4_655 Mgp22 . Fep23 1_655 139.07(4)    yes
O11 4_655 Mgp22 . Fep23 4_555 40.93(4)    yes
Fep23 1_655 Mgp22 . Fep23 4_555 179.996    yes
O11 4_655 Mgp22 . Fep23 4_655 88.82(4)    yes
Fep23 1_655 Mgp22 . Fep23 4_655 60.971(18)    yes
Fep23 4_555 Mgp22 . Fep23 4_655 119.029(18)    yes
O11 4_655 Mgp22 . Om29 . 85.67(6)    yes
Fep23 1_655 Mgp22 . Om29 . 135.27(4)    yes
Fep23 4_555 Mgp22 . Om29 . 44.73(4)    yes
Fep23 4_655 Mgp22 . Om29 . 139.35(4)    yes
O11 4_655 Mgp22 . O9 . 85.67(6)    yes
Fep23 1_655 Mgp22 . O9 . 135.27(4)    yes
Fep23 4_555 Mgp22 . O9 . 44.73(4)    yes
Fep23 4_655 Mgp22 . O9 . 139.35(4)    yes
O11 4_655 Mgp22 . Om210 . 83.78(5)    yes
Fep23 1_655 Mgp22 . Om210 . 89.56(4)    yes
Fep23 4_555 Mgp22 . Om210 . 90.44(4)    yes
Fep23 4_655 Mgp22 . Om210 . 42.16(4)    yes
Om29 . Mgp22 . Om210 . 97.19(6)    yes
O11 4_655 Mgp22 . O10 . 83.78(5)    yes
Fep23 1_655 Mgp22 . O10 . 89.56(4)    yes
Fep23 4_555 Mgp22 . O10 . 90.44(4)    yes
Fep23 4_655 Mgp22 . O10 . 42.16(4)    yes
Om29 . Mgp22 . O10 . 97.19(6)    yes
O11 4_655 Mgp22 . Om211 . 179.995    yes
Fep23 1_655 Mgp22 . Om211 . 40.93(4)    yes
Fep23 4_555 Mgp22 . Om211 . 139.07(4)    yes
Fep23 4_655 Mgp22 . Om211 . 91.18(4)    yes
Om29 . Mgp22 . Om211 . 94.33(6)    yes
O11 4_655 Mgp22 . O11 . 179.995    yes
Fep23 1_655 Mgp22 . O11 . 40.93(4)    yes
Fep23 4_555 Mgp22 . O11 . 139.07(4)    yes
Fep23 4_655 Mgp22 . O11 . 91.18(4)    yes
Om29 . Mgp22 . O11 . 94.33(6)    yes
O9 . Mgp22 . Om210 . 97.19(6)    yes
O9 . Mgp22 . O10 . 97.19(6)    yes
O9 . Mgp22 . Om211 . 94.33(6)    yes
Om210 . Mgp22 . Om211 . 96.22(5)    yes
O10 . Mgp22 . Om211 . 96.22(5)    yes
O9 . Mgp22 . O11 . 94.33(6)    yes
Om210 . Mgp22 . O11 . 96.22(5)    yes
O10 . Mgp22 . O11 . 96.22(5)    yes
O11 4_655 Fep22 . Om29 4_655 94.33(6)    yes
Om211 4_655 Fep22 . Om29 4_655 94.33(6)    yes
O11 4_655 Fep22 . O9 4_655 94.33(6)    yes
Om211 4_655 Fep22 . O9 4_655 94.33(6)    yes
O11 4_655 Fep22 . Om210 4_655 96.22(5)    yes
Om211 4_655 Fep22 . Om210 4_655 96.22(5)    yes
Om29 4_655 Fep22 . Om210 4_655 97.19(6)    yes
O9 4_655 Fep22 . Om210 4_655 97.19(6)    yes
O11 4_655 Fep22 . O10 4_655 96.22(5)    yes
Om211 4_655 Fep22 . O10 4_655 96.22(5)    yes
Om29 4_655 Fep22 . O10 4_655 97.19(6)    yes
O9 4_655 Fep22 . O10 4_655 97.19(6)    yes
O11 4_655 Fep22 . Fep23 1_655 139.07(4)    yes
Om211 4_655 Fep22 . Fep23 1_655 139.07(4)    yes
Om29 4_655 Fep22 . Fep23 1_655 44.73(4)    yes
O9 4_655 Fep22 . Fep23 1_655 44.73(4)    yes
Om210 4_655 Fep22 . Fep23 1_655 90.44(4)    yes
O11 4_655 Fep22 . Fep23 4_555 40.93(4)    yes
Om211 4_655 Fep22 . Fep23 4_555 40.93(4)    yes
Om29 4_655 Fep22 . Fep23 4_555 135.27(4)    yes
O9 4_655 Fep22 . Fep23 4_555 135.27(4)    yes
Om210 4_655 Fep22 . Fep23 4_555 89.56(4)    yes
O11 4_655 Fep22 . Fep23 4_655 88.82(4)    yes
Om211 4_655 Fep22 . Fep23 4_655 88.82(4)    yes
Om29 4_655 Fep22 . Fep23 4_655 40.65(4)    yes
O9 4_655 Fep22 . Fep23 4_655 40.65(4)    yes
Om210 4_655 Fep22 . Fep23 4_655 137.84(4)    yes
O11 4_655 Fep22 . Mgp23 1_655 139.07(4)    yes
Om211 4_655 Fep22 . Mgp23 1_655 139.07(4)    yes
Om29 4_655 Fep22 . Mgp23 1_655 44.73(4)    yes
O9 4_655 Fep22 . Mgp23 1_655 44.73(4)    yes
Om210 4_655 Fep22 . Mgp23 1_655 90.44(4)    yes
O11 4_655 Fep22 . Mgp23 4_555 40.93(4)    yes
Om211 4_655 Fep22 . Mgp23 4_555 40.93(4)    yes
Om29 4_655 Fep22 . Mgp23 4_555 135.27(4)    yes
O9 4_655 Fep22 . Mgp23 4_555 135.27(4)    yes
Om210 4_655 Fep22 . Mgp23 4_555 89.56(4)    yes
O11 4_655 Fep22 . Mgp23 4_655 88.82(4)    yes
Om211 4_655 Fep22 . Mgp23 4_655 88.82(4)    yes
Om29 4_655 Fep22 . Mgp23 4_655 40.65(4)    yes
O9 4_655 Fep22 . Mgp23 4_655 40.65(4)    yes
Om210 4_655 Fep22 . Mgp23 4_655 137.84(4)    yes
O11 4_655 Fep22 . Sip44 . 100.20(4)    yes
Om211 4_655 Fep22 . Sip44 . 100.20(4)    yes
Om29 4_655 Fep22 . Sip44 . 154.19(4)    yes
O9 4_655 Fep22 . Sip44 . 154.19(4)    yes
Om210 4_655 Fep22 . Sip44 . 102.26(4)    yes
O11 4_655 Fep22 . Si4 . 100.20(4)    yes
Om211 4_655 Fep22 . Si4 . 100.20(4)    yes
Om29 4_655 Fep22 . Si4 . 154.19(4)    yes
O9 4_655 Fep22 . Si4 . 154.19(4)    yes
Om210 4_655 Fep22 . Si4 . 102.26(4)    yes
O11 4_655 Fep22 . Sip45 . 99.05(4)    yes
Om211 4_655 Fep22 . Sip45 . 99.05(4)    yes
Om29 4_655 Fep22 . Sip45 . 100.75(4)    yes
O9 4_655 Fep22 . Sip45 . 100.75(4)    yes
Om210 4_655 Fep22 . Sip45 . 155.40(4)    yes
O11 4_655 Fep22 . Si5 . 99.05(4)    yes
Om211 4_655 Fep22 . Si5 . 99.05(4)    yes
Om29 4_655 Fep22 . Si5 . 100.75(4)    yes
O9 4_655 Fep22 . Si5 . 100.75(4)    yes
Om210 4_655 Fep22 . Si5 . 155.40(4)    yes
O11 4_655 Fep22 . Om29 . 85.67(6)    yes
Om211 4_655 Fep22 . Om29 . 85.67(6)    yes
Om29 4_655 Fep22 . Om29 . 179.995    yes
O9 4_655 Fep22 . Om29 . 179.995    yes
Om210 4_655 Fep22 . Om29 . 82.81(6)    yes
O11 4_655 Fep22 . O9 . 85.67(6)    yes
Om211 4_655 Fep22 . O9 . 85.67(6)    yes
Om29 4_655 Fep22 . O9 . 179.995    yes
O9 4_655 Fep22 . O9 . 179.995    yes
Om210 4_655 Fep22 . O9 . 82.81(6)    yes
O11 4_655 Fep22 . Om210 . 83.78(5)    yes
Om211 4_655 Fep22 . Om210 . 83.78(5)    yes
Om29 4_655 Fep22 . Om210 . 82.81(6)    yes
O9 4_655 Fep22 . Om210 . 82.81(6)    yes
Om210 4_655 Fep22 . Om210 . 179.994    yes
O11 4_655 Fep22 . O10 . 83.78(5)    yes
Om211 4_655 Fep22 . O10 . 83.78(5)    yes
Om29 4_655 Fep22 . O10 . 82.81(6)    yes
O9 4_655 Fep22 . O10 . 82.81(6)    yes
Om210 4_655 Fep22 . O10 . 179.994    yes
O11 4_655 Fep22 . Om211 . 179.995    yes
Om211 4_655 Fep22 . Om211 . 179.995    yes
Om29 4_655 Fep22 . Om211 . 85.67(6)    yes
O9 4_655 Fep22 . Om211 . 85.67(6)    yes
Om210 4_655 Fep22 . Om211 . 83.78(5)    yes
O11 4_655 Fep22 . O11 . 179.995    yes
Om211 4_655 Fep22 . O11 . 179.995    yes
Om29 4_655 Fep22 . O11 . 85.67(6)    yes
O9 4_655 Fep22 . O11 . 85.67(6)    yes
Om210 4_655 Fep22 . O11 . 83.78(5)    yes
O10 4_655 Fep22 . Fep23 1_655 90.44(4)    yes
O10 4_655 Fep22 . Fep23 4_555 89.56(4)    yes
Fep23 1_655 Fep22 . Fep23 4_555 179.996    yes
O10 4_655 Fep22 . Fep23 4_655 137.84(4)    yes
Fep23 1_655 Fep22 . Fep23 4_655 60.971(18)    yes
Fep23 4_555 Fep22 . Fep23 4_655 119.029(18)    yes
O10 4_655 Fep22 . Mgp23 1_655 90.44(4)    yes
Fep23 4_555 Fep22 . Mgp23 1_655 179.996    yes
Fep23 4_655 Fep22 . Mgp23 1_655 60.971(18)    yes
O10 4_655 Fep22 . Mgp23 4_555 89.56(4)    yes
Fep23 1_655 Fep22 . Mgp23 4_555 179.996    yes
Fep23 4_655 Fep22 . Mgp23 4_555 119.029(18)    yes
Mgp23 1_655 Fep22 . Mgp23 4_555 179.996    yes
O10 4_655 Fep22 . Mgp23 4_655 137.84(4)    yes
Fep23 1_655 Fep22 . Mgp23 4_655 60.971(18)    yes
Fep23 4_555 Fep22 . Mgp23 4_655 119.029(18)    yes
Mgp23 1_655 Fep22 . Mgp23 4_655 60.971(18)    yes
O10 4_655 Fep22 . Sip44 . 102.26(4)    yes
Fep23 1_655 Fep22 . Sip44 . 117.767(14)    yes
Fep23 4_555 Fep22 . Sip44 . 62.233(14)    yes
Fep23 4_655 Fep22 . Sip44 . 118.019(14)    yes
Mgp23 1_655 Fep22 . Sip44 . 117.767(14)    yes
O10 4_655 Fep22 . Si4 . 102.26(4)    yes
Fep23 1_655 Fep22 . Si4 . 117.767(14)    yes
Fep23 4_555 Fep22 . Si4 . 62.233(14)    yes
Fep23 4_655 Fep22 . Si4 . 118.019(14)    yes
Mgp23 1_655 Fep22 . Si4 . 117.767(14)    yes
O10 4_655 Fep22 . Sip45 . 155.40(4)    yes
Fep23 1_655 Fep22 . Sip45 . 90.552(13)    yes
Fep23 4_555 Fep22 . Sip45 . 89.448(13)    yes
Fep23 4_655 Fep22 . Sip45 . 61.921(13)    yes
Mgp23 1_655 Fep22 . Sip45 . 90.552(13)    yes
O10 4_655 Fep22 . Si5 . 155.40(4)    yes
Fep23 1_655 Fep22 . Si5 . 90.552(13)    yes
Fep23 4_555 Fep22 . Si5 . 89.448(13)    yes
Fep23 4_655 Fep22 . Si5 . 61.921(13)    yes
Mgp23 1_655 Fep22 . Si5 . 90.552(13)    yes
O10 4_655 Fep22 . Om29 . 82.81(6)    yes
Fep23 1_655 Fep22 . Om29 . 135.27(4)    yes
Fep23 4_555 Fep22 . Om29 . 44.73(4)    yes
Fep23 4_655 Fep22 . Om29 . 139.35(4)    yes
Mgp23 1_655 Fep22 . Om29 . 135.27(4)    yes
O10 4_655 Fep22 . O9 . 82.81(6)    yes
Fep23 1_655 Fep22 . O9 . 135.27(4)    yes
Fep23 4_555 Fep22 . O9 . 44.73(4)    yes
Fep23 4_655 Fep22 . O9 . 139.35(4)    yes
Mgp23 1_655 Fep22 . O9 . 135.27(4)    yes
O10 4_655 Fep22 . Om210 . 179.994    yes
Fep23 1_655 Fep22 . Om210 . 89.56(4)    yes
Fep23 4_555 Fep22 . Om210 . 90.44(4)    yes
Fep23 4_655 Fep22 . Om210 . 42.16(4)    yes
Mgp23 1_655 Fep22 . Om210 . 89.56(4)    yes
O10 4_655 Fep22 . O10 . 179.994    yes
Fep23 1_655 Fep22 . O10 . 89.56(4)    yes
Fep23 4_555 Fep22 . O10 . 90.44(4)    yes
Fep23 4_655 Fep22 . O10 . 42.16(4)    yes
Mgp23 1_655 Fep22 . O10 . 89.56(4)    yes
O10 4_655 Fep22 . Om211 . 83.78(5)    yes
Fep23 1_655 Fep22 . Om211 . 40.93(4)    yes
Fep23 4_555 Fep22 . Om211 . 139.07(4)    yes
Fep23 4_655 Fep22 . Om211 . 91.18(4)    yes
Mgp23 1_655 Fep22 . Om211 . 40.93(4)    yes
O10 4_655 Fep22 . O11 . 83.78(5)    yes
Fep23 1_655 Fep22 . O11 . 40.93(4)    yes
Fep23 4_555 Fep22 . O11 . 139.07(4)    yes
Fep23 4_655 Fep22 . O11 . 91.18(4)    yes
Mgp23 1_655 Fep22 . O11 . 40.93(4)    yes
Mgp23 4_555 Fep22 . Mgp23 4_655 119.029(18)    yes
Mgp23 4_555 Fep22 . Sip44 . 62.233(14)    yes
Mgp23 4_655 Fep22 . Sip44 . 118.019(14)    yes
Mgp23 4_555 Fep22 . Si4 . 62.233(14)    yes
Mgp23 4_655 Fep22 . Si4 . 118.019(14)    yes
Mgp23 4_555 Fep22 . Sip45 . 89.448(13)    yes
Mgp23 4_655 Fep22 . Sip45 . 61.921(13)    yes
Sip44 . Fep22 . Sip45 . 56.098(14)    yes
Si4 . Fep22 . Sip45 . 56.098(14)    yes
Mgp23 4_555 Fep22 . Si5 . 89.448(13)    yes
Mgp23 4_655 Fep22 . Si5 . 61.921(13)    yes
Sip44 . Fep22 . Si5 . 56.098(14)    yes
Si4 . Fep22 . Si5 . 56.098(14)    yes
Mgp23 4_555 Fep22 . Om29 . 44.73(4)    yes
Mgp23 4_655 Fep22 . Om29 . 139.35(4)    yes
Sip44 . Fep22 . Om29 . 25.81(4)    yes
Si4 . Fep22 . Om29 . 25.81(4)    yes
Sip45 . Fep22 . Om29 . 79.25(4)    yes
Mgp23 4_555 Fep22 . O9 . 44.73(4)    yes
Mgp23 4_655 Fep22 . O9 . 139.35(4)    yes
Sip44 . Fep22 . O9 . 25.81(4)    yes
Si4 . Fep22 . O9 . 25.81(4)    yes
Sip45 . Fep22 . O9 . 79.25(4)    yes
Mgp23 4_555 Fep22 . Om210 . 90.44(4)    yes
Mgp23 4_655 Fep22 . Om210 . 42.16(4)    yes
Sip44 . Fep22 . Om210 . 77.74(4)    yes
Si4 . Fep22 . Om210 . 77.74(4)    yes
Sip45 . Fep22 . Om210 . 24.60(4)    yes
Mgp23 4_555 Fep22 . O10 . 90.44(4)    yes
Mgp23 4_655 Fep22 . O10 . 42.16(4)    yes
Sip44 . Fep22 . O10 . 77.74(4)    yes
Si4 . Fep22 . O10 . 77.74(4)    yes
Sip45 . Fep22 . O10 . 24.60(4)    yes
Mgp23 4_555 Fep22 . Om211 . 139.07(4)    yes
Mgp23 4_655 Fep22 . Om211 . 91.18(4)    yes
Sip44 . Fep22 . Om211 . 79.80(4)    yes
Si4 . Fep22 . Om211 . 79.80(4)    yes
Sip45 . Fep22 . Om211 . 80.95(4)    yes
Mgp23 4_555 Fep22 . O11 . 139.07(4)    yes
Mgp23 4_655 Fep22 . O11 . 91.18(4)    yes
Sip44 . Fep22 . O11 . 79.80(4)    yes
Si4 . Fep22 . O11 . 79.80(4)    yes
Sip45 . Fep22 . O11 . 80.95(4)    yes
Si5 . Fep22 . Om29 . 79.25(4)    yes
Si5 . Fep22 . O9 . 79.25(4)    yes
Si5 . Fep22 . Om210 . 24.60(4)    yes
Om29 . Fep22 . Om210 . 97.19(6)    yes
O9 . Fep22 . Om210 . 97.19(6)    yes
Si5 . Fep22 . O10 . 24.60(4)    yes
Om29 . Fep22 . O10 . 97.19(6)    yes
O9 . Fep22 . O10 . 97.19(6)    yes
Si5 . Fep22 . Om211 . 80.95(4)    yes
Om29 . Fep22 . Om211 . 94.33(6)    yes
O9 . Fep22 . Om211 . 94.33(6)    yes
Om210 . Fep22 . Om211 . 96.22(5)    yes
O10 . Fep22 . Om211 . 96.22(5)    yes
Si5 . Fep22 . O11 . 80.95(4)    yes
Om29 . Fep22 . O11 . 94.33(6)    yes
O9 . Fep22 . O11 . 94.33(6)    yes
Om210 . Fep22 . O11 . 96.22(5)    yes
O10 . Fep22 . O11 . 96.22(5)    yes
Om211 2_655 Mgp23 . O11 1_455 82.82(7)    yes
O11 2_655 Mgp23 . O11 1_455 82.82(7)    yes
Om211 2_655 Mgp23 . Om211 1_455 82.82(7)    yes
O11 2_655 Mgp23 . Om211 1_455 82.82(7)    yes
Om211 2_655 Mgp23 . O10 4_655 97.68(6)    yes
O11 2_655 Mgp23 . O10 4_655 97.68(6)    yes
O11 1_455 Mgp23 . O10 4_655 178.98(6)    yes
Om211 1_455 Mgp23 . O10 4_655 178.98(6)    yes
Om211 2_655 Mgp23 . Om210 4_655 97.68(6)    yes
O11 2_655 Mgp23 . Om210 4_655 97.68(6)    yes
O11 1_455 Mgp23 . Om210 4_655 178.98(6)    yes
Om211 1_455 Mgp23 . Om210 4_655 178.98(6)    yes
Om211 2_655 Mgp23 . O10 3_445 85.61(6)    yes
O11 2_655 Mgp23 . O10 3_445 85.61(6)    yes
O11 1_455 Mgp23 . O10 3_445 95.53(6)    yes
Om211 1_455 Mgp23 . O10 3_445 95.53(6)    yes
O10 4_655 Mgp23 . O10 3_445 85.40(6)    yes
Om211 2_655 Mgp23 . Om210 3_445 85.61(6)    yes
O11 2_655 Mgp23 . Om210 3_445 85.61(6)    yes
O11 1_455 Mgp23 . Om210 3_445 95.53(6)    yes
Om211 1_455 Mgp23 . Om210 3_445 95.53(6)    yes
O10 4_655 Mgp23 . Om210 3_445 85.40(6)    yes
Om211 2_655 Mgp23 . O9 4_555 97.34(5)    yes
O11 2_655 Mgp23 . O9 4_555 97.34(5)    yes
O11 1_455 Mgp23 . O9 4_555 87.45(6)    yes
Om211 1_455 Mgp23 . O9 4_555 87.45(6)    yes
O10 4_655 Mgp23 . O9 4_555 91.60(6)    yes
Om211 2_655 Mgp23 . Om29 4_555 97.34(5)    yes
O11 2_655 Mgp23 . Om29 4_555 97.34(5)    yes
O11 1_455 Mgp23 . Om29 4_555 87.45(6)    yes
Om211 1_455 Mgp23 . Om29 4_555 87.45(6)    yes
O10 4_655 Mgp23 . Om29 4_555 91.60(6)    yes
Om211 2_655 Mgp23 . Fep23 2_555 42.27(4)    yes
O11 2_655 Mgp23 . Fep23 2_555 42.27(4)    yes
O11 1_455 Mgp23 . Fep23 2_555 40.56(5)    yes
Om211 1_455 Mgp23 . Fep23 2_555 40.56(5)    yes
O10 4_655 Mgp23 . Fep23 2_555 139.94(5)    yes
Om211 2_655 Mgp23 . Fep22 1_455 90.26(4)    yes
O11 2_655 Mgp23 . Fep22 1_455 90.26(4)    yes
O11 1_455 Mgp23 . Fep22 1_455 43.89(5)    yes
Om211 1_455 Mgp23 . Fep22 1_455 43.89(5)    yes
O10 4_655 Mgp23 . Fep22 1_455 135.16(5)    yes
Om211 2_655 Mgp23 . Om29 . 178.91(6)    yes
O11 2_655 Mgp23 . Om29 . 178.91(6)    yes
O11 1_455 Mgp23 . Om29 . 97.82(6)    yes
Om211 1_455 Mgp23 . Om29 . 97.82(6)    yes
O10 4_655 Mgp23 . Om29 . 81.69(6)    yes
Om211 2_655 Mgp23 . O9 . 178.91(6)    yes
O11 2_655 Mgp23 . O9 . 178.91(6)    yes
O11 1_455 Mgp23 . O9 . 97.82(6)    yes
Om211 1_455 Mgp23 . O9 . 97.82(6)    yes
O10 4_655 Mgp23 . O9 . 81.69(6)    yes
Om210 4_655 Mgp23 . O10 3_445 85.40(6)    yes
Om210 4_655 Mgp23 . Om210 3_445 85.40(6)    yes
Om210 4_655 Mgp23 . O9 4_555 91.60(6)    yes
O10 3_445 Mgp23 . O9 4_555 176.06(6)    yes
Om210 3_445 Mgp23 . O9 4_555 176.06(6)    yes
Om210 4_655 Mgp23 . Om29 4_555 91.60(6)    yes
O10 3_445 Mgp23 . Om29 4_555 176.06(6)    yes
Om210 3_445 Mgp23 . Om29 4_555 176.06(6)    yes
Om210 4_655 Mgp23 . Fep23 2_555 139.94(5)    yes
O10 3_445 Mgp23 . Fep23 2_555 90.87(5)    yes
Om210 3_445 Mgp23 . Fep23 2_555 90.87(5)    yes
O9 4_555 Mgp23 . Fep23 2_555 93.07(4)    yes
Om29 4_555 Mgp23 . Fep23 2_555 93.07(4)    yes
Om210 4_655 Mgp23 . Fep22 1_455 135.16(5)    yes
O10 3_445 Mgp23 . Fep22 1_455 139.35(4)    yes
Om210 3_445 Mgp23 . Fep22 1_455 139.35(4)    yes
O9 4_555 Mgp23 . Fep22 1_455 43.56(4)    yes
Om29 4_555 Mgp23 . Fep22 1_455 43.56(4)    yes
Om210 4_655 Mgp23 . Om29 . 81.69(6)    yes
O10 3_445 Mgp23 . Om29 . 93.45(5)    yes
Om210 3_445 Mgp23 . Om29 . 93.45(5)    yes
O9 4_555 Mgp23 . Om29 . 83.57(6)    yes
Om29 4_555 Mgp23 . Om29 . 83.57(6)    yes
Om210 4_655 Mgp23 . O9 . 81.69(6)    yes
O10 3_445 Mgp23 . O9 . 93.45(5)    yes
Om210 3_445 Mgp23 . O9 . 93.45(5)    yes
O9 4_555 Mgp23 . O9 . 83.57(6)    yes
Om29 4_555 Mgp23 . O9 . 83.57(6)    yes
Fep23 2_555 Mgp23 . Fep22 1_455 60.949(15)    yes
Fep23 2_555 Mgp23 . Om29 . 138.37(5)    yes
Fep22 1_455 Mgp23 . Om29 . 90.81(4)    yes
Fep23 2_555 Mgp23 . O9 . 138.37(5)    yes
Fep22 1_455 Mgp23 . O9 . 90.81(4)    yes
O9 4_555 Fep23 . Om210 3_445 176.06(6)    yes
Om29 4_555 Fep23 . Om210 3_445 176.06(6)    yes
O9 4_555 Fep23 . O10 3_445 176.06(6)    yes
Om29 4_555 Fep23 . O10 3_445 176.06(6)    yes
O9 4_555 Fep23 . O10 4_655 91.60(6)    yes
Om29 4_555 Fep23 . O10 4_655 91.60(6)    yes
Om210 3_445 Fep23 . O10 4_655 85.40(6)    yes
O10 3_445 Fep23 . O10 4_655 85.40(6)    yes
O9 4_555 Fep23 . Om210 4_655 91.60(6)    yes
Om29 4_555 Fep23 . Om210 4_655 91.60(6)    yes
Om210 3_445 Fep23 . Om210 4_655 85.40(6)    yes
O10 3_445 Fep23 . Om210 4_655 85.40(6)    yes
O9 4_555 Fep23 . Fep23 2_555 93.07(4)    yes
Om29 4_555 Fep23 . Fep23 2_555 93.07(4)    yes
Om210 3_445 Fep23 . Fep23 2_555 90.87(5)    yes
O10 3_445 Fep23 . Fep23 2_555 90.87(5)    yes
O10 4_655 Fep23 . Fep23 2_555 139.94(5)    yes
O9 4_555 Fep23 . Fep22 1_455 43.56(4)    yes
Om29 4_555 Fep23 . Fep22 1_455 43.56(4)    yes
Om210 3_445 Fep23 . Fep22 1_455 139.35(4)    yes
O10 3_445 Fep23 . Fep22 1_455 139.35(4)    yes
O10 4_655 Fep23 . Fep22 1_455 135.16(5)    yes
O9 4_555 Fep23 . O11 1_455 87.45(6)    yes
Om29 4_555 Fep23 . O11 1_455 87.45(6)    yes
Om210 3_445 Fep23 . O11 1_455 95.53(6)    yes
O10 3_445 Fep23 . O11 1_455 95.53(6)    yes
O10 4_655 Fep23 . O11 1_455 178.98(6)    yes
O9 4_555 Fep23 . Om211 1_455 87.45(6)    yes
Om29 4_555 Fep23 . Om211 1_455 87.45(6)    yes
Om210 3_445 Fep23 . Om211 1_455 95.53(6)    yes
O10 3_445 Fep23 . Om211 1_455 95.53(6)    yes
O10 4_655 Fep23 . Om211 1_455 178.98(6)    yes
O9 4_555 Fep23 . Om211 2_655 97.34(5)    yes
Om29 4_555 Fep23 . Om211 2_655 97.34(5)    yes
Om210 3_445 Fep23 . Om211 2_655 85.61(6)    yes
O10 3_445 Fep23 . Om211 2_655 85.61(6)    yes
O10 4_655 Fep23 . Om211 2_655 97.68(6)    yes
O9 4_555 Fep23 . Om29 . 83.57(6)    yes
Om29 4_555 Fep23 . Om29 . 83.57(6)    yes
Om210 3_445 Fep23 . Om29 . 93.45(5)    yes
O10 3_445 Fep23 . Om29 . 93.45(5)    yes
O10 4_655 Fep23 . Om29 . 81.69(6)    yes
O9 4_555 Fep23 . O9 . 83.57(6)    yes
Om29 4_555 Fep23 . O9 . 83.57(6)    yes
Om210 3_445 Fep23 . O9 . 93.45(5)    yes
O10 3_445 Fep23 . O9 . 93.45(5)    yes
O10 4_655 Fep23 . O9 . 81.69(6)    yes
Om210 4_655 Fep23 . Fep23 2_555 139.94(5)    yes
Om210 4_655 Fep23 . Fep22 1_455 135.16(5)    yes
Fep23 2_555 Fep23 . Fep22 1_455 60.949(15)    yes
Om210 4_655 Fep23 . O11 1_455 178.98(6)    yes
Fep23 2_555 Fep23 . O11 1_455 40.56(5)    yes
Fep22 1_455 Fep23 . O11 1_455 43.89(5)    yes
Om210 4_655 Fep23 . Om211 1_455 178.98(6)    yes
Fep23 2_555 Fep23 . Om211 1_455 40.56(5)    yes
Fep22 1_455 Fep23 . Om211 1_455 43.89(5)    yes
Om210 4_655 Fep23 . Om211 2_655 97.68(6)    yes
Fep23 2_555 Fep23 . Om211 2_655 42.27(4)    yes
Fep22 1_455 Fep23 . Om211 2_655 90.26(4)    yes
O11 1_455 Fep23 . Om211 2_655 82.82(7)    yes
Om211 1_455 Fep23 . Om211 2_655 82.82(7)    yes
Om210 4_655 Fep23 . Om29 . 81.69(6)    yes
Fep23 2_555 Fep23 . Om29 . 138.37(5)    yes
Fep22 1_455 Fep23 . Om29 . 90.81(4)    yes
O11 1_455 Fep23 . Om29 . 97.82(6)    yes
Om211 1_455 Fep23 . Om29 . 97.82(6)    yes
Om210 4_655 Fep23 . O9 . 81.69(6)    yes
Fep23 2_555 Fep23 . O9 . 138.37(5)    yes
Fep22 1_455 Fep23 . O9 . 90.81(4)    yes
O11 1_455 Fep23 . O9 . 97.82(6)    yes
Om211 1_455 Fep23 . O9 . 97.82(6)    yes
Om211 2_655 Fep23 . Om29 . 178.91(6)    yes
Om211 2_655 Fep23 . O9 . 178.91(6)    yes
Si5 1_455 Sip44 . Fep23 4_555 62.616(17)    yes
Sip45 1_455 Sip44 . Fep23 4_555 62.616(17)    yes
Si5 1_455 Sip44 . Fep22 . 118.02(2)    yes
Sip45 1_455 Sip44 . Fep22 . 118.02(2)    yes
Fep23 4_555 Sip44 . Fep22 . 55.407(13)    yes
Si5 1_455 Sip44 . Sip45 . 119.83(2)    yes
Sip45 1_455 Sip44 . Sip45 . 119.83(2)    yes
Fep23 4_555 Sip44 . Sip45 . 88.90(2)    yes
Fep22 . Sip44 . Sip45 . 61.981(17)    yes
Si5 1_455 Sip44 . Si5 . 119.83(2)    yes
Sip45 1_455 Sip44 . Si5 . 119.83(2)    yes
Fep23 4_555 Sip44 . Si5 . 88.90(2)    yes
Fep22 . Sip44 . Si5 . 61.981(17)    yes
Si5 1_455 Sip44 . Om26 . 124.11(7)    yes
Sip45 1_455 Sip44 . Om26 . 124.11(7)    yes
Fep23 4_555 Sip44 . Om26 . 109.36(7)    yes
Fep22 . Sip44 . Om26 . 79.64(7)    yes
Sip45 . Sip44 . Om26 . 21.18(6)    yes
Si5 1_455 Sip44 . O6 . 124.11(7)    yes
Sip45 1_455 Sip44 . O6 . 124.11(7)    yes
Fep23 4_555 Sip44 . O6 . 109.36(7)    yes
Fep22 . Sip44 . O6 . 79.64(7)    yes
Sip45 . Sip44 . O6 . 21.18(6)    yes
Si5 1_455 Sip44 . Om27 . 21.70(6)    yes
Sip45 1_455 Sip44 . Om27 . 21.70(6)    yes
Fep23 4_555 Sip44 . Om27 . 80.78(7)    yes
Fep22 . Sip44 . Om27 . 134.81(7)    yes
Sip45 . Sip44 . Om27 . 111.70(7)    yes
Si5 1_455 Sip44 . O7 . 21.70(6)    yes
Sip45 1_455 Sip44 . O7 . 21.70(6)    yes
Fep23 4_555 Sip44 . O7 . 80.78(7)    yes
Fep22 . Sip44 . O7 . 134.81(7)    yes
Sip45 . Sip44 . O7 . 111.70(7)    yes
Si5 1_455 Sip44 . Om28 . 111.95(6)    yes
Sip45 1_455 Sip44 . Om28 . 111.95(6)    yes
Fep23 4_555 Sip44 . Om28 . 135.56(6)    yes
Fep22 . Sip44 . Om28 . 110.76(6)    yes
Sip45 . Sip44 . Om28 . 123.92(6)    yes
Si5 1_455 Sip44 . O8 . 111.95(6)    yes
Sip45 1_455 Sip44 . O8 . 111.95(6)    yes
Fep23 4_555 Sip44 . O8 . 135.56(6)    yes
Fep22 . Sip44 . O8 . 110.76(6)    yes
Sip45 . Sip44 . O8 . 123.92(6)    yes
Si5 1_455 Sip44 . Om29 . 91.17(6)    yes
Sip45 1_455 Sip44 . Om29 . 91.17(6)    yes
Fep23 4_555 Sip44 . Om29 . 35.29(6)    yes
Fep22 . Sip44 . Om29 . 33.38(5)    yes
Sip45 . Sip44 . Om29 . 91.83(5)    yes
Si5 1_455 Sip44 . O9 . 91.17(6)    yes
Sip45 1_455 Sip44 . O9 . 91.17(6)    yes
Fep23 4_555 Sip44 . O9 . 35.29(6)    yes
Fep22 . Sip44 . O9 . 33.38(5)    yes
Sip45 . Sip44 . O9 . 91.83(5)    yes
Si5 . Sip44 . Om26 . 21.18(6)    yes
Si5 . Sip44 . O6 . 21.18(6)    yes
Si5 . Sip44 . Om27 . 111.70(7)    yes
Om26 . Sip44 . Om27 . 108.60(10)    yes
O6 . Sip44 . Om27 . 108.60(10)    yes
Si5 . Sip44 . O7 . 111.70(7)    yes
Om26 . Sip44 . O7 . 108.60(10)    yes
O6 . Sip44 . O7 . 108.60(10)    yes
Si5 . Sip44 . Om28 . 123.92(6)    yes
Om26 . Sip44 . Om28 . 108.36(9)    yes
O6 . Sip44 . Om28 . 108.36(9)    yes
Om27 . Sip44 . Om28 . 108.28(9)    yes
O7 . Sip44 . Om28 . 108.28(9)    yes
Si5 . Sip44 . O8 . 123.92(6)    yes
Om26 . Sip44 . O8 . 108.36(9)    yes
O6 . Sip44 . O8 . 108.36(9)    yes
Om27 . Sip44 . O8 . 108.28(9)    yes
O7 . Sip44 . O8 . 108.28(9)    yes
Si5 . Sip44 . Om29 . 91.83(5)    yes
Om26 . Sip44 . Om29 . 111.61(8)    yes
O6 . Sip44 . Om29 . 111.61(8)    yes
Om27 . Sip44 . Om29 . 112.20(9)    yes
O7 . Sip44 . Om29 . 112.20(9)    yes
Si5 . Sip44 . O9 . 91.83(5)    yes
Om26 . Sip44 . O9 . 111.61(8)    yes
O6 . Sip44 . O9 . 111.61(8)    yes
Om27 . Sip44 . O9 . 112.20(9)    yes
O7 . Sip44 . O9 . 112.20(9)    yes
Om28 . Sip44 . Om29 . 107.66(9)    yes
O8 . Sip44 . Om29 . 107.66(9)    yes
Om28 . Sip44 . O9 . 107.66(9)    yes
O8 . Sip44 . O9 . 107.66(9)    yes
Si5 1_455 Si4 . Fep23 4_555 62.616(17)    yes
Sip45 1_455 Si4 . Fep23 4_555 62.616(17)    yes
Si5 1_455 Si4 . Fep22 . 118.02(2)    yes
Sip45 1_455 Si4 . Fep22 . 118.02(2)    yes
Fep23 4_555 Si4 . Fep22 . 55.407(13)    yes
Si5 1_455 Si4 . Sip45 . 119.83(2)    yes
Sip45 1_455 Si4 . Sip45 . 119.83(2)    yes
Fep23 4_555 Si4 . Sip45 . 88.90(2)    yes
Fep22 . Si4 . Sip45 . 61.981(17)    yes
Si5 1_455 Si4 . Si5 . 119.83(2)    yes
Sip45 1_455 Si4 . Si5 . 119.83(2)    yes
Fep23 4_555 Si4 . Si5 . 88.90(2)    yes
Fep22 . Si4 . Si5 . 61.981(17)    yes
Si5 1_455 Si4 . Om26 . 124.11(7)    yes
Sip45 1_455 Si4 . Om26 . 124.11(7)    yes
Fep23 4_555 Si4 . Om26 . 109.36(7)    yes
Fep22 . Si4 . Om26 . 79.64(7)    yes
Sip45 . Si4 . Om26 . 21.18(6)    yes
Si5 1_455 Si4 . O6 . 124.11(7)    yes
Sip45 1_455 Si4 . O6 . 124.11(7)    yes
Fep23 4_555 Si4 . O6 . 109.36(7)    yes
Fep22 . Si4 . O6 . 79.64(7)    yes
Sip45 . Si4 . O6 . 21.18(6)    yes
Si5 1_455 Si4 . Om27 . 21.70(6)    yes
Sip45 1_455 Si4 . Om27 . 21.70(6)    yes
Fep23 4_555 Si4 . Om27 . 80.78(7)    yes
Fep22 . Si4 . Om27 . 134.81(7)    yes
Sip45 . Si4 . Om27 . 111.70(7)    yes
Si5 1_455 Si4 . O7 . 21.70(6)    yes
Sip45 1_455 Si4 . O7 . 21.70(6)    yes
Fep23 4_555 Si4 . O7 . 80.78(7)    yes
Fep22 . Si4 . O7 . 134.81(7)    yes
Sip45 . Si4 . O7 . 111.70(7)    yes
Si5 1_455 Si4 . Om28 . 111.95(6)    yes
Sip45 1_455 Si4 . Om28 . 111.95(6)    yes
Fep23 4_555 Si4 . Om28 . 135.56(6)    yes
Fep22 . Si4 . Om28 . 110.76(6)    yes
Sip45 . Si4 . Om28 . 123.92(6)    yes
Si5 1_455 Si4 . O8 . 111.95(6)    yes
Sip45 1_455 Si4 . O8 . 111.95(6)    yes
Fep23 4_555 Si4 . O8 . 135.56(6)    yes
Fep22 . Si4 . O8 . 110.76(6)    yes
Sip45 . Si4 . O8 . 123.92(6)    yes
Si5 1_455 Si4 . Om29 . 91.17(6)    yes
Sip45 1_455 Si4 . Om29 . 91.17(6)    yes
Fep23 4_555 Si4 . Om29 . 35.29(6)    yes
Fep22 . Si4 . Om29 . 33.38(5)    yes
Sip45 . Si4 . Om29 . 91.83(5)    yes
Si5 1_455 Si4 . O9 . 91.17(6)    yes
Sip45 1_455 Si4 . O9 . 91.17(6)    yes
Fep23 4_555 Si4 . O9 . 35.29(6)    yes
Fep22 . Si4 . O9 . 33.38(5)    yes
Sip45 . Si4 . O9 . 91.83(5)    yes
Si5 . Si4 . Om26 . 21.18(6)    yes
Si5 . Si4 . O6 . 21.18(6)    yes
Si5 . Si4 . Om27 . 111.70(7)    yes
Om26 . Si4 . Om27 . 108.60(10)    yes
O6 . Si4 . Om27 . 108.60(10)    yes
Si5 . Si4 . O7 . 111.70(7)    yes
Om26 . Si4 . O7 . 108.60(10)    yes
O6 . Si4 . O7 . 108.60(10)    yes
Si5 . Si4 . Om28 . 123.92(6)    yes
Om26 . Si4 . Om28 . 108.36(9)    yes
O6 . Si4 . Om28 . 108.36(9)    yes
Om27 . Si4 . Om28 . 108.28(9)    yes
O7 . Si4 . Om28 . 108.28(9)    yes
Si5 . Si4 . O8 . 123.92(6)    yes
Om26 . Si4 . O8 . 108.36(9)    yes
O6 . Si4 . O8 . 108.36(9)    yes
Om27 . Si4 . O8 . 108.28(9)    yes
O7 . Si4 . O8 . 108.28(9)    yes
Si5 . Si4 . Om29 . 91.83(5)    yes
Om26 . Si4 . Om29 . 111.61(8)    yes
O6 . Si4 . Om29 . 111.61(8)    yes
Om27 . Si4 . Om29 . 112.20(9)    yes
O7 . Si4 . Om29 . 112.20(9)    yes
Si5 . Si4 . O9 . 91.83(5)    yes
Om26 . Si4 . O9 . 111.61(8)    yes
O6 . Si4 . O9 . 111.61(8)    yes
Om27 . Si4 . O9 . 112.20(9)    yes
O7 . Si4 . O9 . 112.20(9)    yes
Om28 . Si4 . Om29 . 107.66(9)    yes
O8 . Si4 . Om29 . 107.66(9)    yes
Om28 . Si4 . O9 . 107.66(9)    yes
O8 . Si4 . O9 . 107.66(9)    yes
Om27 1_655 Sip45 . Om28 3_555 108.59(9)    yes
O7 1_655 Sip45 . Om28 3_555 108.59(9)    yes
Om27 1_655 Sip45 . O8 3_555 108.59(9)    yes
O7 1_655 Sip45 . O8 3_555 108.59(9)    yes
Om27 1_655 Sip45 . Si4 1_655 21.69(7)    yes
O7 1_655 Sip45 . Si4 1_655 21.69(7)    yes
Om28 3_555 Sip45 . Si4 1_655 124.27(6)    yes
O8 3_555 Sip45 . Si4 1_655 124.27(6)    yes
Om27 1_655 Sip45 . Sip44 1_655 21.69(7)    yes
O7 1_655 Sip45 . Sip44 1_655 21.69(7)    yes
Om28 3_555 Sip45 . Sip44 1_655 124.27(6)    yes
O8 3_555 Sip45 . Sip44 1_655 124.27(6)    yes
Om27 1_655 Sip45 . Si4 . 123.69(7)    yes
O7 1_655 Sip45 . Si4 . 123.69(7)    yes
Om28 3_555 Sip45 . Si4 . 111.60(6)    yes
O8 3_555 Sip45 . Si4 . 111.60(6)    yes
Si4 1_655 Sip45 . Si4 . 119.83(2)    yes
Om27 1_655 Sip45 . Sip44 . 123.69(7)    yes
O7 1_655 Sip45 . Sip44 . 123.69(7)    yes
Om28 3_555 Sip45 . Sip44 . 111.60(6)    yes
O8 3_555 Sip45 . Sip44 . 111.60(6)    yes
Si4 1_655 Sip45 . Sip44 . 119.83(2)    yes
Om27 1_655 Sip45 . Fep23 3_555 135.70(7)    yes
O7 1_655 Sip45 . Fep23 3_555 135.70(7)    yes
Om28 3_555 Sip45 . Fep23 3_555 80.73(6)    yes
O8 3_555 Sip45 . Fep23 3_555 80.73(6)    yes
Si4 1_655 Sip45 . Fep23 3_555 118.61(2)    yes
Om27 1_655 Sip45 . Fep22 . 110.69(7)    yes
O7 1_655 Sip45 . Fep22 . 110.69(7)    yes
Om28 3_555 Sip45 . Fep22 . 134.69(6)    yes
O8 3_555 Sip45 . Fep22 . 134.69(6)    yes
Si4 1_655 Sip45 . Fep22 . 89.899(19)    yes
Om27 1_655 Sip45 . Om26 . 108.15(10)    yes
O7 1_655 Sip45 . Om26 . 108.15(10)    yes
Om28 3_555 Sip45 . Om26 . 108.56(9)    yes
O8 3_555 Sip45 . Om26 . 108.56(9)    yes
Si4 1_655 Sip45 . Om26 . 111.53(7)    yes
Om27 1_655 Sip45 . O6 . 108.15(10)    yes
O7 1_655 Sip45 . O6 . 108.15(10)    yes
Om28 3_555 Sip45 . O6 . 108.56(9)    yes
O8 3_555 Sip45 . O6 . 108.56(9)    yes
Si4 1_655 Sip45 . O6 . 111.53(7)    yes
Om27 1_655 Sip45 . Om210 . 109.38(8)    yes
O7 1_655 Sip45 . Om210 . 109.38(8)    yes
Om28 3_555 Sip45 . Om210 . 113.39(9)    yes
O8 3_555 Sip45 . Om210 . 113.39(9)    yes
Si4 1_655 Sip45 . Om210 . 88.41(5)    yes
Om27 1_655 Sip45 . O10 . 109.38(8)    yes
O7 1_655 Sip45 . O10 . 109.38(8)    yes
Om28 3_555 Sip45 . O10 . 113.39(9)    yes
O8 3_555 Sip45 . O10 . 113.39(9)    yes
Si4 1_655 Sip45 . O10 . 88.41(5)    yes
Sip44 1_655 Sip45 . Si4 . 119.83(2)    yes
Sip44 1_655 Sip45 . Sip44 . 119.83(2)    yes
Sip44 1_655 Sip45 . Fep23 3_555 118.61(2)    yes
Si4 . Sip45 . Fep23 3_555 88.86(2)    yes
Sip44 . Sip45 . Fep23 3_555 88.86(2)    yes
Sip44 1_655 Sip45 . Fep22 . 89.899(19)    yes
Si4 . Sip45 . Fep22 . 61.921(16)    yes
Sip44 . Sip45 . Fep22 . 61.921(16)    yes
Fep23 3_555 Sip45 . Fep22 . 55.370(13)    yes
Sip44 1_655 Sip45 . Om26 . 111.53(7)    yes
Si4 . Sip45 . Om26 . 21.18(6)    yes
Sip44 . Sip45 . Om26 . 21.18(6)    yes
Fep23 3_555 Sip45 . Om26 . 109.32(7)    yes
Fep22 . Sip45 . Om26 . 79.58(7)    yes
Sip44 1_655 Sip45 . O6 . 111.53(7)    yes
Si4 . Sip45 . O6 . 21.18(6)    yes
Sip44 . Sip45 . O6 . 21.18(6)    yes
Fep23 3_555 Sip45 . O6 . 109.32(7)    yes
Fep22 . Sip45 . O6 . 79.58(7)    yes
Sip44 1_655 Sip45 . Om210 . 88.41(5)    yes
Si4 . Sip45 . Om210 . 88.85(6)    yes
Sip44 . Sip45 . Om210 . 88.85(6)    yes
Fep23 3_555 Sip45 . Om210 . 35.21(6)    yes
Fep22 . Sip45 . Om210 . 30.72(6)    yes
Sip44 1_655 Sip45 . O10 . 88.41(5)    yes
Si4 . Sip45 . O10 . 88.85(6)    yes
Sip44 . Sip45 . O10 . 88.85(6)    yes
Fep23 3_555 Sip45 . O10 . 35.21(6)    yes
Fep22 . Sip45 . O10 . 30.72(6)    yes
Om26 . Sip45 . Om210 . 108.64(9)    yes
O6 . Sip45 . Om210 . 108.64(9)    yes
Om26 . Sip45 . O10 . 108.64(9)    yes
O6 . Sip45 . O10 . 108.64(9)    yes
Om27 1_655 Si5 . Om28 3_555 108.59(9)    yes
O7 1_655 Si5 . Om28 3_555 108.59(9)    yes
Om27 1_655 Si5 . O8 3_555 108.59(9)    yes
O7 1_655 Si5 . O8 3_555 108.59(9)    yes
Om27 1_655 Si5 . Si4 1_655 21.69(7)    yes
O7 1_655 Si5 . Si4 1_655 21.69(7)    yes
Om28 3_555 Si5 . Si4 1_655 124.27(6)    yes
O8 3_555 Si5 . Si4 1_655 124.27(6)    yes
Om27 1_655 Si5 . Sip44 1_655 21.69(7)    yes
O7 1_655 Si5 . Sip44 1_655 21.69(7)    yes
Om28 3_555 Si5 . Sip44 1_655 124.27(6)    yes
O8 3_555 Si5 . Sip44 1_655 124.27(6)    yes
Om27 1_655 Si5 . Si4 . 123.69(7)    yes
O7 1_655 Si5 . Si4 . 123.69(7)    yes
Om28 3_555 Si5 . Si4 . 111.60(6)    yes
O8 3_555 Si5 . Si4 . 111.60(6)    yes
Si4 1_655 Si5 . Si4 . 119.83(2)    yes
Om27 1_655 Si5 . Sip44 . 123.69(7)    yes
O7 1_655 Si5 . Sip44 . 123.69(7)    yes
Om28 3_555 Si5 . Sip44 . 111.60(6)    yes
O8 3_555 Si5 . Sip44 . 111.60(6)    yes
Si4 1_655 Si5 . Sip44 . 119.83(2)    yes
Om27 1_655 Si5 . Fep23 3_555 135.70(7)    yes
O7 1_655 Si5 . Fep23 3_555 135.70(7)    yes
Om28 3_555 Si5 . Fep23 3_555 80.73(6)    yes
O8 3_555 Si5 . Fep23 3_555 80.73(6)    yes
Si4 1_655 Si5 . Fep23 3_555 118.61(2)    yes
Om27 1_655 Si5 . Fep22 . 110.69(7)    yes
O7 1_655 Si5 . Fep22 . 110.69(7)    yes
Om28 3_555 Si5 . Fep22 . 134.69(6)    yes
O8 3_555 Si5 . Fep22 . 134.69(6)    yes
Si4 1_655 Si5 . Fep22 . 89.899(19)    yes
Om27 1_655 Si5 . Om26 . 108.15(10)    yes
O7 1_655 Si5 . Om26 . 108.15(10)    yes
Om28 3_555 Si5 . Om26 . 108.56(9)    yes
O8 3_555 Si5 . Om26 . 108.56(9)    yes
Si4 1_655 Si5 . Om26 . 111.53(7)    yes
Om27 1_655 Si5 . O6 . 108.15(10)    yes
O7 1_655 Si5 . O6 . 108.15(10)    yes
Om28 3_555 Si5 . O6 . 108.56(9)    yes
O8 3_555 Si5 . O6 . 108.56(9)    yes
Si4 1_655 Si5 . O6 . 111.53(7)    yes
Om27 1_655 Si5 . Om210 . 109.38(8)    yes
O7 1_655 Si5 . Om210 . 109.38(8)    yes
Om28 3_555 Si5 . Om210 . 113.39(9)    yes
O8 3_555 Si5 . Om210 . 113.39(9)    yes
Si4 1_655 Si5 . Om210 . 88.41(5)    yes
Om27 1_655 Si5 . O10 . 109.38(8)    yes
O7 1_655 Si5 . O10 . 109.38(8)    yes
Om28 3_555 Si5 . O10 . 113.39(9)    yes
O8 3_555 Si5 . O10 . 113.39(9)    yes
Si4 1_655 Si5 . O10 . 88.41(5)    yes
Sip44 1_655 Si5 . Si4 . 119.83(2)    yes
Sip44 1_655 Si5 . Sip44 . 119.83(2)    yes
Sip44 1_655 Si5 . Fep23 3_555 118.61(2)    yes
Si4 . Si5 . Fep23 3_555 88.86(2)    yes
Sip44 . Si5 . Fep23 3_555 88.86(2)    yes
Sip44 1_655 Si5 . Fep22 . 89.899(19)    yes
Si4 . Si5 . Fep22 . 61.921(16)    yes
Sip44 . Si5 . Fep22 . 61.921(16)    yes
Fep23 3_555 Si5 . Fep22 . 55.370(13)    yes
Sip44 1_655 Si5 . Om26 . 111.53(7)    yes
Si4 . Si5 . Om26 . 21.18(6)    yes
Sip44 . Si5 . Om26 . 21.18(6)    yes
Fep23 3_555 Si5 . Om26 . 109.32(7)    yes
Fep22 . Si5 . Om26 . 79.58(7)    yes
Sip44 1_655 Si5 . O6 . 111.53(7)    yes
Si4 . Si5 . O6 . 21.18(6)    yes
Sip44 . Si5 . O6 . 21.18(6)    yes
Fep23 3_555 Si5 . O6 . 109.32(7)    yes
Fep22 . Si5 . O6 . 79.58(7)    yes
Sip44 1_655 Si5 . Om210 . 88.41(5)    yes
Si4 . Si5 . Om210 . 88.85(6)    yes
Sip44 . Si5 . Om210 . 88.85(6)    yes
Fep23 3_555 Si5 . Om210 . 35.21(6)    yes
Fep22 . Si5 . Om210 . 30.72(6)    yes
Sip44 1_655 Si5 . O10 . 88.41(5)    yes
Si4 . Si5 . O10 . 88.85(6)    yes
Sip44 . Si5 . O10 . 88.85(6)    yes
Fep23 3_555 Si5 . O10 . 35.21(6)    yes
Fep22 . Si5 . O10 . 30.72(6)    yes
Om26 . Si5 . Om210 . 108.64(9)    yes
O6 . Si5 . Om210 . 108.64(9)    yes
Om26 . Si5 . O10 . 108.64(9)    yes
O6 . Si5 . O10 . 108.64(9)    yes
Si5 . Om26 . Si4 . 137.63(12)    yes
Sip45 . Om26 . Si4 . 137.63(12)    yes
Si5 . Om26 . Sip44 . 137.63(12)    yes
Sip45 . Om26 . Sip44 . 137.63(12)    yes
Si5 . O6 . Si4 . 137.63(12)    yes
Sip45 . O6 . Si4 . 137.63(12)    yes
Si5 . O6 . Sip44 . 137.63(12)    yes
Sip45 . O6 . Sip44 . 137.63(12)    yes
Si5 1_455 Om27 . Si4 . 136.61(12)    yes
Sip45 1_455 Om27 . Si4 . 136.61(12)    yes
Si5 1_455 Om27 . Sip44 . 136.61(12)    yes
Sip45 1_455 Om27 . Sip44 . 136.61(12)    yes
Si5 1_455 O7 . Si4 . 136.61(12)    yes
Sip45 1_455 O7 . Si4 . 136.61(12)    yes
Si5 1_455 O7 . Sip44 . 136.61(12)    yes
Sip45 1_455 O7 . Sip44 . 136.61(12)    yes
Si5 3_445 Om28 . Si4 . 136.62(10)    yes
Sip45 3_445 Om28 . Si4 . 136.62(10)    yes
Si5 3_445 Om28 . Sip44 . 136.62(10)    yes
Sip45 3_445 Om28 . Sip44 . 136.62(10)    yes
Si5 3_445 O8 . Si4 . 136.62(10)    yes
Sip45 3_445 O8 . Si4 . 136.62(10)    yes
Si5 3_445 O8 . Sip44 . 136.62(10)    yes
Sip45 3_445 O8 . Sip44 . 136.62(10)    yes
Fep23 4_555 Om29 . Fep22 . 91.71(6)    yes
Fep23 4_555 Om29 . Mgp23 . 96.43(6)    yes
Fep22 . Om29 . Mgp23 . 97.76(6)    yes
Fep23 4_555 Om29 . Fep23 . 96.43(6)    yes
Fep22 . Om29 . Fep23 . 97.76(6)    yes
Fep23 4_555 Om29 . Mgp22 . 91.71(6)    yes
Mgp23 . Om29 . Mgp22 . 97.76(6)    yes
Fep23 . Om29 . Mgp22 . 97.76(6)    yes
Fep22 . Om29 . Mgp23 4_555 91.71(6)    yes
Mgp23 . Om29 . Mgp23 4_555 96.43(6)    yes
Fep23 . Om29 . Mgp23 4_555 96.43(6)    yes
Mgp22 . Om29 . Mgp23 4_555 91.71(6)    yes
Fep23 4_555 Om29 . Sip44 . 118.12(9)    yes
Fep22 . Om29 . Sip44 . 120.81(7)    yes
Mgp23 . Om29 . Sip44 . 124.80(9)    yes
Fep23 . Om29 . Sip44 . 124.80(9)    yes
Mgp22 . Om29 . Sip44 . 120.81(7)    yes
Fep23 4_555 Om29 . Si4 . 118.12(9)    yes
Fep22 . Om29 . Si4 . 120.81(7)    yes
Mgp23 . Om29 . Si4 . 124.80(9)    yes
Fep23 . Om29 . Si4 . 124.80(9)    yes
Mgp22 . Om29 . Si4 . 120.81(7)    yes
Mgp23 4_555 Om29 . Sip44 . 118.12(9)    yes
Mgp23 4_555 Om29 . Si4 . 118.12(9)    yes
Fep23 4_555 O9 . Fep22 . 91.71(6)    yes
Fep23 4_555 O9 . Mgp23 . 96.43(6)    yes
Fep22 . O9 . Mgp23 . 97.76(6)    yes
Fep23 4_555 O9 . Fep23 . 96.43(6)    yes
Fep22 . O9 . Fep23 . 97.76(6)    yes
Fep23 4_555 O9 . Mgp22 . 91.71(6)    yes
Mgp23 . O9 . Mgp22 . 97.76(6)    yes
Fep23 . O9 . Mgp22 . 97.76(6)    yes
Fep22 . O9 . Mgp23 4_555 91.71(6)    yes
Mgp23 . O9 . Mgp23 4_555 96.43(6)    yes
Fep23 . O9 . Mgp23 4_555 96.43(6)    yes
Mgp22 . O9 . Mgp23 4_555 91.71(6)    yes
Fep23 4_555 O9 . Sip44 . 118.12(9)    yes
Fep22 . O9 . Sip44 . 120.81(7)    yes
Mgp23 . O9 . Sip44 . 124.80(9)    yes
Fep23 . O9 . Sip44 . 124.80(9)    yes
Mgp22 . O9 . Sip44 . 120.81(7)    yes
Fep23 4_555 O9 . Si4 . 118.12(9)    yes
Fep22 . O9 . Si4 . 120.81(7)    yes
Mgp23 . O9 . Si4 . 124.80(9)    yes
Fep23 . O9 . Si4 . 124.80(9)    yes
Mgp22 . O9 . Si4 . 120.81(7)    yes
Mgp23 4_555 O9 . Sip44 . 118.12(9)    yes
Mgp23 4_555 O9 . Si4 . 118.12(9)    yes
Fep23 3_555 Om210 . Fep23 4_655 94.60(6)    yes
Fep23 3_555 Om210 . Mgp22 . 93.46(5)    yes
Fep23 4_655 Om210 . Mgp22 . 97.74(6)    yes
Fep23 3_555 Om210 . Fep22 . 93.46(5)    yes
Fep23 4_655 Om210 . Fep22 . 97.74(6)    yes
Fep23 3_555 Om210 . Mgp23 4_655 94.60(6)    yes
Mgp22 . Om210 . Mgp23 4_655 97.74(6)    yes
Fep22 . Om210 . Mgp23 4_655 97.74(6)    yes
Fep23 4_655 Om210 . Mgp23 3_555 94.60(6)    yes
Mgp22 . Om210 . Mgp23 3_555 93.46(5)    yes
Fep22 . Om210 . Mgp23 3_555 93.46(5)    yes
Mgp23 4_655 Om210 . Mgp23 3_555 94.60(6)    yes
Fep23 3_555 Om210 . Sip45 . 118.26(9)    yes
Fep23 4_655 Om210 . Sip45 . 121.08(7)    yes
Mgp22 . Om210 . Sip45 . 124.67(9)    yes
Fep22 . Om210 . Sip45 . 124.67(9)    yes
Mgp23 4_655 Om210 . Sip45 . 121.08(7)    yes
Fep23 3_555 Om210 . Si5 . 118.26(9)    yes
Fep23 4_655 Om210 . Si5 . 121.08(7)    yes
Mgp22 . Om210 . Si5 . 124.67(9)    yes
Fep22 . Om210 . Si5 . 124.67(9)    yes
Mgp23 4_655 Om210 . Si5 . 121.08(7)    yes
Mgp23 3_555 Om210 . Sip45 . 118.26(9)    yes
Mgp23 3_555 Om210 . Si5 . 118.26(9)    yes
Fep23 3_555 O10 . Fep23 4_655 94.60(6)    yes
Fep23 3_555 O10 . Mgp22 . 93.46(5)    yes
Fep23 4_655 O10 . Mgp22 . 97.74(6)    yes
Fep23 3_555 O10 . Fep22 . 93.46(5)    yes
Fep23 4_655 O10 . Fep22 . 97.74(6)    yes
Fep23 3_555 O10 . Mgp23 4_655 94.60(6)    yes
Mgp22 . O10 . Mgp23 4_655 97.74(6)    yes
Fep22 . O10 . Mgp23 4_655 97.74(6)    yes
Fep23 4_655 O10 . Mgp23 3_555 94.60(6)    yes
Mgp22 . O10 . Mgp23 3_555 93.46(5)    yes
Fep22 . O10 . Mgp23 3_555 93.46(5)    yes
Mgp23 4_655 O10 . Mgp23 3_555 94.60(6)    yes
Fep23 3_555 O10 . Sip45 . 118.26(9)    yes
Fep23 4_655 O10 . Sip45 . 121.08(7)    yes
Mgp22 . O10 . Sip45 . 124.67(9)    yes
Fep22 . O10 . Sip45 . 124.67(9)    yes
Mgp23 4_655 O10 . Sip45 . 121.08(7)    yes
Fep23 3_555 O10 . Si5 . 118.26(9)    yes
Fep23 4_655 O10 . Si5 . 121.08(7)    yes
Mgp22 . O10 . Si5 . 124.67(9)    yes
Fep22 . O10 . Si5 . 124.67(9)    yes
Mgp23 4_655 O10 . Si5 . 121.08(7)    yes
Mgp23 3_555 O10 . Sip45 . 118.26(9)    yes
Mgp23 3_555 O10 . Si5 . 118.26(9)    yes
Mgp23 2_655 Om211 . Mgp23 1_655 97.18(7)    yes
Mgp23 2_655 Om211 . Fep22 . 97.15(6)    yes
Mgp23 1_655 Om211 . Fep22 . 95.17(6)    yes
Mgp23 2_655 Om211 . Mgp22 . 97.15(6)    yes
Mgp23 1_655 Om211 . Mgp22 . 95.17(6)    yes
Mgp23 2_655 Om211 . Fep23 1_655 97.18(7)    yes
Fep22 . Om211 . Fep23 1_655 95.17(6)    yes
Mgp22 . Om211 . Fep23 1_655 95.17(6)    yes
Mgp23 1_655 Om211 . Fep23 2_655 97.18(7)    yes
Fep22 . Om211 . Fep23 2_655 97.15(6)    yes
Mgp22 . Om211 . Fep23 2_655 97.15(6)    yes
Fep23 1_655 Om211 . Fep23 2_655 97.18(7)    yes
Mgp23 2_655 O11 . Mgp23 1_655 97.18(7)    yes
Mgp23 2_655 O11 . Fep22 . 97.15(6)    yes
Mgp23 1_655 O11 . Fep22 . 95.17(6)    yes
Mgp23 2_655 O11 . Mgp22 . 97.15(6)    yes
Mgp23 1_655 O11 . Mgp22 . 95.17(6)    yes
Mgp23 2_655 O11 . Fep23 1_655 97.18(7)    yes
Fep22 . O11 . Fep23 1_655 95.17(6)    yes
Mgp22 . O11 . Fep23 1_655 95.17(6)    yes
Mgp23 1_655 O11 . Fep23 2_655 97.18(7)    yes
Fep22 . O11 . Fep23 2_655 97.15(6)    yes
Mgp22 . O11 . Fep23 2_655 97.15(6)    yes
Fep23 1_655 O11 . Fep23 2_655 97.18(7)    yes


_iucr_refine_instruction_details_constraints
;
#
# Punched on 20/06/11 at 16:33:02
#
#LIST     12                                                                    
FULL 
CONT  KP1(1,OCC) UNTIL FEP2(3) 
CONT KP1(1,Y) 
CONT KP1(1, U[11], U[22], U[33], U[13]) 
RIDE MGP2 (2, U'S) FEP2 (2, U'S) 
RIDE MGP2 (3, X'S, U'S) FEP2 (3, X'S, U'S) 
RIDE SIP4(4,OCC, X'S,U'S) SI(4,OCC, X'S,U'S) 
WEIGHT -1 SI(4,OCC) 
RIDE SIP4(5,OCC, X'S,U'S) SI(5,OCC, X'S,U'S) 
WEIGHT -1 SI(5,OCC) 
RIDE OM2(6,OCC, X'S,U'S) O(6,OCC,X'S,U'S) 
WEIGHT -1 O(6, OCC) 
RIDE OM2(7,OCC, X'S,U'S) O(7,OCC, X'S,U'S) 
WEIGHT -1 O(7, OCC) 
RIDE OM2(8,OCC, X'S,U'S) O(8,OCC, X'S,U'S) 
WEIGHT -1 O(8, OCC) 
RIDE OM2(9,OCC, X'S,U'S) O(9,OCC, X'S,U'S) 
WEIGHT -1 O(9, OCC) 
RIDE OM2(10,OCC, X'S,U'S) O(10,OCC, X'S,U'S) 
WEIGHT -1 O(10, OCC) 
RIDE OM2(11,OCC, X'S,U'S) O(11,OCC, X'S,U'S) 
WEIGHT -1 O(11, OCC) 
END                                                                             
;


_iucr_refine_instruction_details_restraints
;
#
# Punched on 20/06/11 at 16:33:02
#
#LIST     16                                                                    
RESTR 0.5, 0.2 = KP1(1,OCC) 
RESTR .50, .001 =  MGP2(2,OCC)+ FEP2(2,OCC) 
RESTR 1.0,.001 = MGP2(3,OCC)+FEP2(3,OCC) 
LIMIT 0.001 OCC 
END                                                                             
;
